Proc. Nat. Acad. Sci. USA Vol. 73, No. 4, pp. 988-989, April 1976 Chemistry
Viscosity of liquid metals: An interpretation (fluidity of liquid metals/solubility parameters) J. H. HILDEBRAND AND R. H. LAMOREAUX Department of Chemistry, University of California, Berkeley, Calif. 94720 Contributed by Joel H. Hildebrand, January 9, 1976
ABSTRACT The fluidity of liquid metals, like that of that this is the case with many of the metals in Table 1. In simple nonmetallic liquids, is a linear function of the ratio of the cases of Ga, Sb, and Bi, which expand on freezing, V. is, unoccupied volume to intrinsic volume over long ranges as of course, larger than Vo. Their fields of force are not sym- expressed by the equation X = B[(V/Vo) - 1J. Values of Vo obtained by extrapolating to = 0 agree well with molal vol- metrical; Ga crystals are orthorhombic and those of Sb and umes of compact crystals at 200C calculated from densities. Bi are rhombohedral. Values of the ratio 0/[( V/Vo) - 1] range from 27.0 for Na The purpose of this paper is not to consider change of vol- to 1.55 reciprocal centipoise for Ni. Viscosities at ratios of ex- ume on freezing but only to show that the parameter VO de- pansion V/V0 = 1.10 vary linearly with squares of solubility rived from fluidity at high temperatures represents a real parameters AE"/Vo, where AE" is molal energy of vaporiza- physical quantity, the intrinsic volume of a mole of close- tion at the melting point. Viscosities at 10% expansion range packed, highly symmetrical molecules, appropriate for our from 0.037 cP for Na to 5.38 cP for Co, with some divergence for metals with values of q in the neighborhood of unity. The purpose of dealing with the viscosity of liquids. good agreement in the case of the transition metals Cu, Fe, In order to study the factors that are embodied in the con- Co, and Ni we attribute to distribution of vector momentum stant B of Eq. 1, we have plotted in Fig. 1 values of X versus among quasi-chemical bonds between d-electrons and vacant (V/Vo) - 1 for each metal. Values of the slopes, given in orbitals. Table 1, give the fluidities at equal expansions over intrinsic volumes. Their enormous range, from 27 to 1.55, invites the- We have shown in a series papers of (1-5) that fluidity X) oretical analysis. Lines for the non-metals, Ne, CH4, SiCl4, (the reciprocal of viscosity, a) of simple liquids is a linear and C12, have been included for comparison. Their slopes function of their molal volumes V over considerable ranges decrease with liquid heat capacities (5). It is striking that the of temperature pressure as and expressed by the simple points for alkali metals other than Li all fall on the same equation: line, the steepest with fluidity far higher than that of any = B[(V/Vo) - 1]  Table 1. Values of parameters The intercept of the X-V line at = 0 is the intrinsic, close- constant B packed molal volume. The proportionality is ) AEV largest for symmetric, elastic molecules that do not transpose vector momentum into rotational or vibrational energy. The VO Vs V/VO-1 VO 7? purpose of this paper is to examine the applicability of these concepts to an understanding of the viscosity of liquid met- 1 Li 12.4 13.0 14.5 2.9 0.07 als. 2 Na 24.5 24.1 27.0 0.56 0.04 3 K 44.2 45.4 27.0 0.45 0.04 Data on the viscosities of liquid metals over ranges of tem- 4 Rb 55.3 55.8 27.0 - perature are given in the Landolt-Bornstein Tables To (6). 5 Mg "13 14.0 -3.5 2.3 molal volumes over of we used calculate ranges temperature 6 Ca -23 26.3 -3.1 1.6 the extensive compilation by Cowley (7). 7 Al 10.7 10.0 11.0 7.2 0.91 We obtained lines that are quite straight, except at high 8 Fe 7.05 7.05 2.04 12.3 4.9 temperatures in a few cases to be discussed. Extrapolation to 9 Co 6.80 6.80 1.86 12.7 5.4 V0 at = 0 involves a considerable interval in the lines for 10 Ni 6.70 6.70 1.55 13.8 6.5 Mg and Ca, consequently the precision of a value of Vo is 11 Cu 7.10 7.14 2.3 9.8 4.4 limited by the length of this interval, the range of measure- 12 Zn 9.50 9.45 5.7 2.7 1.8 ments, and the scatter of points. Our values of Vo are listed 13 Ag 11.0 10.28 3.9 6.1 2.56 in Table 1. They differ a little from corresponding values 14 Cd 13.0 13.0 5.0 1.7 2.0 obtained by Wittenberg and DeWitt (8) in an important 15 Hg 14.1 14.14 11.9 2.0 0.84 paper on changes of volume on melting, mainly because we 16 Ga 11.1 11.8 15.0 0.67 used a different source for the dependence of volume upon 17 In 15.7 15.8 12.5 3.5 0.80 temperature. 18 Sn 16.4 16.3 13.0 4.1 0.77 In the second column of figures in Table 1 we give values 19 Pb 18.8 18.3 8.8 2.3 1.14 of the molal volumes of the solid metals at 20'C, calculated 20 Sb 17.6 18.4 10.6 0.94 from densities given in the American Physical Society 21 Bi 19.6 21.4 9.8 4.5 1.0 Handbook vary, some cases of Physics (8). These values in 4 is fluidity in reciprocal centipoise, cP-1 (1 P = 1 g cm-' sec-'). by as much as 2%, depending upon the method of preparing V is volume in cm3 mo1l'. Vo is its value at X = 0; V. is its value the sample or whether calculated from x-ray-determined di- for the solid at 20'C. AEv is energy of vaporization in kcal mol-1 mensions. We discussed in reference 2 the conditions under (1 kcal = 4.184 kJ) of the liquid metal at its melting point. s7 is which Vo and Vs, might have the same value. It is striking viscosity, in cP, of liquid metal when V/V0 = 1.10. 988 Downloaded by guest on September 24, 2021 Chemistry: Hildebrand and Lamoreaux Proc. Nat. Acad. Sci. USA 73 (1976) 989
10. 6 9
0 4 -
14 3 12 0. 2 * 19 21 150 . 7 17 *I E0c2,3 5 'I.10 15 AEvV/o V kcal CM-3 mol-
FIG. 2. Viscosity, i7, cP, at liquid expansion V/VO-1 = 0.100 against cohesion expressed by molal energy of vaporization per cm3 at the melting point, kcal cm-3 mol-1. Numbers relate the V/VO - I points to the elements in Table 1.
FIG. 1. Fluidity of liquid metals, X in cP-1, against ratios of free volume to occupied volume. momentum. Perhaps viscosity has more to teach than to learn about these interactions. not same other metals and much less than that of CH4 at the We thank colleagues Leo Brewer, Kenneth Pitzer, and John degree of expansion. This seems consistent with the fact that Prausnitz for helpful discussions of this subject. the atom of each of these metals possesses a single valence electron in symmetrical s-orbital. 1. Hildebrand, J. H. (1971) "Motions of molecules in liquids," Let us view the same data from the standpoint of viscosi- Science 174, 490-493. ty, all at the expansion 1.10 V/Vo, plotted as ordinates in 2. Hildebrand, J. H. & Lamoreaux, R. H. (1972) "Fluidity: A gen- Fig. 2. As abscissae are plotted values of molal energy of va- eral theory," Proc. Nat. Acad. Sci. USA 69,3428-3431. porization at melting points divided by V0, AE"/Vo. We 3. Alder, B. J. & Hildebrand, J. H. (1973) "Activation energy: Not involved in transport processes in liquids," Ind. Eng. Chem. have subtracted RT from values of heats of vaporization at Fundam 12,387-388. melting points from Selected Values of the Thermodynamic 4. Hildebrand, J. H. & Lamoreaux, R. H. (1973) "Viscosity along Properties of the Elements (9). AEv/Vo is the square of the continuous paths between liquid and gas," Physica 74, 416- "solubility parameter," 6, now widely used as a measure of 422. cohesion. Applied to liquid metals, it includes not only pure- 5. Hildebrand, J. H. (1975) "Kinetic theory of viscosity of com- ly physical, London dispersion forces, but also the much pressed fluids," Proc. Nat. Acad. Sci. USA 72, 1970-1972. larger quasi-chemical forces between the atoms with d-elec- 6. Landolt-B6rnstein Tabellen (Springer-Verlag, Berlin), II 5a, trons and vacant orbitals in the transition elements, notably p. 124 ff. Cu, Fe, Co, and Ni. 7. Crawley, A. F. (1974) "Densities of liquid metals and alloys," Int. Metall. Rev. (Department of The group of metals with values of AE"/Vo between 2 Energy, Mines and Re- sources, Ottawa, Canada), pp. 32-40. and 4 kcal cm-3 are more molh' considerably viscous than 8. Wittenberg, L. J. & DeWitt, R. (1972) "Volume contraction the alkali metals to some Na Cs, indicating probability of during melting; emphasis on lanthanide and actinide ele- formation of hybrid interatomic orbitals. Our present quan- ments," J. Chem. Phys. 56, 4526-4533. titative knowledge of forces in liquid Sn, In, Hg, Pb, and Al 9. Hultgren, R. (ed.) (1973) Selected Values of the Thermody- seems insufficient to predict their absorbtivity for vector namic Properties of the Elements (Wiley, New York). Downloaded by guest on September 24, 2021